Abstract
Potential crystal structures of BeB_{2} were explored using ab initio evolutionary simulations. A new phase with a Cmcm space group was uncovered. It was determined that the Cmcm phase is mechanically and dynamically stable and has a lower enthalpy, from ambient pressure up to 13 GPa, than any previously proposed phases, as measured using firstprinciples calculations. The crystal structure, phonon dispersion, phase transitions, and mechanical and electronic properties of this phase were investigated. It was determined that the Cmcm phase may transform into the phase at pressures higher than 13 GPa. The band structures and density of states reveal that the Cmcm phase is metallic. In addition, the Vickers hardness was calculated using three empirical models. To explain the origin of the hardness, charge density difference maps and a Mulliken population analysis were carried out, which demonstrated that there are strong covalent interactions between B atoms. By analyzing the Crystal Orbital Hamilton Population (COHP) diagrams, it was determined that the total interaction of the BeB bonds is stronger than that of the BB bonds, indicating a very complex bonding feature in the new phase. It was predicted that the new Cmcm phase is nearly absent of superconductivity.
Introduction
Beryllium (Be) and boron (B) are elements that occupy adjacent positions in the periodic table, but they have quite different properties, as the former is a metal while the latter is a semiconductor under standard conditions. At ambient conditions, Be crystallizes in a hexagonalclosedpacked (hcp) structure and transforms into a body centered cubic (bcc) crystal structure at 1523 K or approximately 400 GPa^{1,2}. It has gained considerable attention because of its simple atomic configuration and unusual behaviors. As it is highly transmissive to Xrays, Be is commonly used as a window material in Xray equipment^{3}. It is also one of the most effective moderators and reflectors for neutrons used in nuclear reactors^{4}. In addition, its light weight, high melting point and highstrength performance result in it being widely used in aircraft, rockets, satellites and other aerospace applications, as well as in future fusion reactors^{5,6}. Although Be has several negative characteristics, such as potential toxicity that poses a manufacturing challenge, controlled handling procedures, such as the use of a glove box, can enable the success industrial synthesis of berylliumcontaining compounds^{7,8}.
Boron is a semiconductor that becomes a metal, and even a superconductor, when placed under high pressure^{9}. Elemental boron has many allotropes that use the B_{12} icosahedron as the basic unit, of which αBoron is the most common^{10}. Boroncontaining compounds have been investigated extensively due to their exotic physical properties, such as superconductivity, hardness and thermoelectric performance. For example, several transition metal diborides, such as OsB_{2}, IrB_{2}, ReB_{2} and BC_{x}, possess high bulk and shear moduli and have been explored for use as potential superhard materials^{11,12,13,14,15,16}.
When beryllium and boron combine, various BeB phases ranging from berylliumrich to boronrich will form. Some Berich phases, such as the Be_{2}B phase, show a metallic character and are potential superconductors^{17}. Another berylliumrich phase, Be_{4}B, is the only stable Berich phase at room temperature. Within the boronrich compounds, BeB_{3}, found only in the MgIn_{3} type (space group , NO.221, one formula unit per cell), is found to be not stable. BeB_{4}, however, is highly stable at high pressures^{2}.
Although beryllium diboride has been known and studied for more than half century^{18,19,20,21,22,23}, there has still been no solid evidence that it exists with the stoichiometry BeB_{2}. The first announced synthesis of BeB_{2.01 ± 0.03} with P6/mmm symmetry^{18} was later recognized to have a correct stoichiometry of BeB_{2.75} with a surprisingly complex crystal structure^{19}. Very recently, Hermann, A. et al. systematically studied the binary BeB phases at ambient and highpressure conditions^{2,20}. In their work, they found that the most stable structure for BeB_{2} at atmospheric pressure is cubic (space group , NO.216), with a diamondoid boron network and beryllium atoms occupying interstitial tetrahedral sites. This structure is semiconducting and can be understood in terms of the ZintlKlemm concept, making it unique among BeB phases. Other proposed beryllium diboron phases can be classified into three crystal systems: (1) cubic, including the CaAl_{2} structure (space group , NO.227, eight units per cell, prototype MgCu_{2}^{24} ) and “AlLiSi” structures (space group , NO.216^{20}); (2) hexagonal, including the MgB_{2} crystal structure (space group P6/mmm, NO.191^{20}, one unit per cell, prototype AlB_{2}) and the CaIn_{2} and MgGa_{2} structures (space group P63/mmc, NO.194, two units per cell^{25,26}); and (3) orthorhombic, including the SrAl_{2} structure (space group Imma, NO.74, four units per cell, prototype CeCu_{2}^{27}), another MgGa_{2} structure (space group Pbam, NO.55, eight units per cell^{28}) and the “CaIn_{2}” structure (space group Pnma, NO.62^{20}). Many phases have already been found. At low pressure (under 160 GPa), the cubic phase (space group , NO.216) is the most stable, while the P63/mmc phase is dynamically unstable and can turn into lowsymmetry Pnma. At pressures greater than 160 GPa, the P63/mmc phase is more stable^{2}. There is still an open question regarding whether there exist other stable phases with low energy in the low pressure zone. Therefore, further theoretical studies, such as of the crystalline structure, electronic properties and mechanical properties, are important for this potential material.
In the present work, potential crystal structures of BeB_{2} were extensively explored using ab initio evolutionary simulations. A new phase with Cmcm symmetry was uncovered. The crystal structures, phonon dispersions, mechanical properties, phase transitions, and electronic structures of this phase as well as other available phases were investigated. The band structures and density of states reveal that the new phase is metallic. Further study on the mechanical properties using three different methods was used to predict the Vickers hardness of the newly discovered Cmcm phase. Charge density difference maps and Mulliken population analysis, as well as COHP diagrams, were also carried out to analyze the character of the bonding between the atoms in Cmcm BeB_{2}. The superconductivity of the new Cmcm phase was also investigated.
Results
Crystal Structure
In a previous work, several phases were found both experimentally and theoretically. However, only four structures are stable according to the calculated phonon spectra in the present work. These are cubic (space group , NO.216), orthorhombic (space group Pnma, NO.62), orthorhombic (space group Pbam, NO.55) and hexagonal (space group P63/mmc, NO.194). In the present work, a new stable phase with space group NO.63 was uncovered by performing systematic structure searches for BeB_{2}. Its optimized equilibrium lattice parameters, axial ratio c/a and unit cell volume are shown in Table 1. The crystal structure information of all other known dynamical stable phases are presented in Table 2^{2,20}. Table 1 reveals that the conventional unit cell of the new Cmcm phase contains twelve atoms in total with two inequivalent Wyckoff positions 4c and 8f for Be and B atoms, respectively.
The schematic crystal structure of the Cmcm phase is shown in Figures 1, 2 and 3, where yellow and blue spheres represent Be and B atoms, respectively. Figure 1 shows the unit cell, while Figure 2 shows the supercell of the same crystal structure. Figure 2(b) is perpendicular to the xaxis. There are two parallel columns formed by boroncentered and berylliumcentered coordination polyhedra that are marked by green and blue colors, respectively. Each boron atom is surrounded by four beryllium atoms that form a distorted tetrahedral configuration. Eight boron atoms embrace a beryllium atom, forming a complex polyhedron composed of 3 rectangles and 6 triangles. Along the zaxis, the structure can be viewed as several layers, as shown in Figure 2 (b) and (c). Six boron atoms connect to each other in a hexagonal ring, where 4 atoms are coplanar (denoted as B and B*) and the other 2 atoms are out of this plane (denoted as A and A*). Be atoms form another layer (denoted as C) between the B and B* layers along the zaxis. The upper image of Figure 2 (a) is taken from the A, B, C, B* and A* layers, whereas the lower image is composed of the B*, A*, C*, A and B layers. The distance between two A layers is 5.120 Å. The configurations of boroncentered and berylliumcentered coordination polyhedra are displayed in Figure 3. The distances of the three types of BeB bonds are 1.923 Å, 2.021 Å and 2.105 Å, respectively, as shown in Figure 3 (a). The BoronBoron bond lengths are 1.763 Å (the blue bond) and 1.657 Å (the green bond), as shown in Figure 3 (b).
Phonon Dispersion
The phonon dispersion curves of the new phase as well as of other previously proposed crystalline structures were calculated to determine their dynamical stability, as shown in Figure 4. The new Cmcm phase is dynamically stable, as there are no imaginary phonon frequencies detected in the whole Brillouin zone. For the previously proposed phases^{2,20}, the Pbam, Pnma, and P63/mmc phases are dynamically stable according to the same rule. However, the appearance of imaginary frequencies indicates that the P6/mmm, and Imma phases mentioned in previously published articles^{2,20} are dynamically unstable.
Phase Transition
Figure 5 gives the calculated relative enthalpy as a function of pressure for all stable phases of BeB_{2}, relative to the phase. The inserted figures show the stable Cmcm phase and the phase of BeB_{2}, before and after the phase transition at 13 GPa, respectively. As mentioned before, the latter has been considered in previous works to be the most stable phase at atmospheric pressure, having a structure with a diamondoid boron network and beryllium atoms occupying the interstitial tetrahedral sites. The polyhedron representation of the phase has also been marked, as shown in the bottomright corner of Figure 5.
As shown in Figure 5, the enthalpy of the newly uncovered phase increases with pressure within the studied pressure range up to 50 GPa, while the enthalpies of the other three stable phases (Pnma phase, Pbam phase, P63/mmc phase) have an inverse trend. It can be concluded that the Cmcm phase is more competitive than the previously known most stable phase at pressures up to 13 GPa. When the pressure exceeds 40 GPa, the Pnma phase and P63/mmc phase have almost similar enthalpies, and both of them become more favorable than the new Cmcm phase. The cubic structure ( phase) continues to have the greatest stability in the pressure range from 13 GPa to 50 GPa. These results are consistent with the results previously found by Andreas Hermann et al.^{2}
Firstprinciples methods were used to calculate the formation enthalpy of the new phase Cmcm (No.63) at different pressures. The structural parameters of each phase are listed in Table 3. The enthalpy of formation is calculated as follows: As shown in Table 4, when the pressure is 1 atm, the formation enthalpy of the Cmcm phase is −56 meV/atom, which is within the range of formation enthalpies (−40 meV to −125 meV) of some proposed models for BeB_{2.79} phases^{20}. This may explain why the BeB_{2.79} phase with a very complex structure has been found experimentally, rather than the pure BeB_{2} phase with the simple Cmcm structure. It also indicates that the proposed models of BeB_{2.79} phases^{20} with enthalpies less than −56 meV/atom are more competitive. Upon comparing the formation enthalpy of the new phase (− 0.056 eV/atom) with that of the most stable known phase (−0.016 eV/atom), it may be observed that the former is more competitive than the latter. In short, the Cmcm phase is more thermodynamically stable than any other known BeB_{2} phase.
Using the same approach, the formation enthalpy of the Cmcm phase at 10 GPa and 15 GPa was calculated to be −39.7 meV/atom and −32.2 meV/atom, respectively. By comparing to the value at 1 atm (−56.267 meV/atom), it may be seen that the formation enthalpy value increases continuously with the pressure, indicating that increasing pressure is not beneficial for the synthesis of the Cmcm phase. All of these conclusions agree well with those obtained from the pressure phase diagram^{2,20}, and the results will provide guidance for experimental work on BeB_{2} synthesis.
In addition, to provide more “physics” of the phase transition, we have calculated the solidsolid structural phase transitions between the Cmcm and phases at 13 GPa by using the VCNEB method^{29}. Figure 6 illustrate the snapshots from a dynamical trajectory collected from transition path sampling connecting the Cmcm phase and the phase. The energy barrier of the transition was calculated to be 0.25 eV/atom.
Discussion
Mechanical Properties
Mechanical properties, including the elastic constants, bulk modulus, shear modulus, Young's modulus, Poisson's ratio, are the main bases for choosing and designing materials. Therefore, all these properties were calculated using the firstprinciples approach in this work. The elastic constants of all structures under the ambient pressure C_{ij} were calculated with the strainstress method combined with Hooke's Law, as implemented in the CASTEP code^{30}. The results are listed in Table 5. In order to determine the mechanical stability of the new predictions, C_{ij} has to satisfy the elastic stability criteria^{31}.
The mechanical stability condition and elastic constants of the orthogonal structure are positive. However, the following inequalities must also be satisfied to indicate stability:
As shown in Table 5, these values all meet the mechanical stability criteria, initially confirming that the Cmcm phase is mechanically stable.
Based on the VoigtReussHill approximation method^{32,33}, we can find the appropriate bulk modulus B and shear modulus G using the elastic constants. In addition, the values of Young's modulus E and Poisson's ratio σ can be calculated using the following formula: Usually, the bulk modulus B is used to characterize a material's resistance to volume deformation against external pressure, while the shear modulus G measures a material's ability to resist shear strain. Young's modulus E measures the resistance against longitudinal tensions. Among the 4 mechanical and dynamical stable BeB_{2} phases, the Cmcm phase has the lowest value of bulk modulus and the second lowest shear modulus, revealing that it has low resistance to compression and shear strain. In addition, the elastic constant C_{22} (282 GPa) is significantly smaller than C_{11} (492 GPa) and C_{33} (690 GPa), revealing that resistance along the b axis is much smaller than along the a and c axes.
In order to evaluate the ductility of the material, the B/G values were calculated and are listed in Table 5. Higher B/G values greater than 1.75 correspond to a ductile material, while values less than 1.75 correspond to a brittle material^{34}. As shown in Table 5, the B/G value of the Cmcm phase is approximately 1.01, suggesting that it is very brittle.
Poisson's ratio reflects the strength of the covalent bond to some extent. A small Poisson's ratio (σ = 0.13) indicates that the Cmcm phase is more intensely covalently linked than the Pbam phase (σ = 0.29) and P63/mmc phase (σ = 0.18). These results show that the Cmcm phase is likely to be a type of potential ultraincompressible material, despite its bulk modulus and shear modulus not being very high.
Finally, the hardness of the Cmcm phase was calculated in three different ways. Using a recently proposed simple empirical hardness formula H_{v} = 2(G^{3}/B^{2})^{0.585}–3^{35}, the Vickers hardness of these phases was calculated. As the result shows, the Cmcm phase has a hardness value of 36.8 GPa, approaching the critical value of a superhard material, 40 GPa. It also reveals that the predicted hardnesses of the Pnma phase and the phase are approximately 41.4 GPa and 42.3 GPa, respectively, implying that both of them are potential superhard materials. The hardness value for the Cmcm phase is also calculated to be 25.2 GPa using th he formula of hardness given by Artem R. Oganov^{36} (details can be found in the computational methods section).
The hardness of the new phase was also calculated by the microscopic hardness model proposed by F.M. Gao et al.^{37,38} (details can be found in the computational methods section). The calculated parameters and hardness of the Cmcm phase calculated by this model are listed in Table 6. It is found that the total hardness of the Cmcm phase is only 13.8 GPa with this method.
Chen's model gives the highest values (36.8 GPa) from these three models followed by Oganov's model (25.2 GPa) while Gao's model provides the lowest values (13.8 GPa), which may be caused by their applicability to the boron compounds and with metals. The scattered values of hardness predicted from these three different models reveal that although it has a simple crystal structure, the electronic structure and bonding characters of the newly uncovered Cmcm phase of BeB_{2} are quite complex, as will be analyzed below.
Electronic Properties
The electronic properties of the newly discovered phase, including energy band structures, total and partial density of states (DOS), and charge density maps, were calculated and are shown in Figure 7,8,9.
Figure 7 shows the calculated band structure along high symmetry directions, as well as the total and partial DOS of the optimized Cmcm structure from firstprinciples calculations within the GGA scheme. The overlapping of the valence bands and conduction bands around the Fermi level suggests that the new phase has a clear metallic character, which is confirmed by the finite value of total DOS at the Fermi level.
Figure 7 also plots the partial DOS of the novel Cmcm phase. It reveals that the total DOS of the upper part of the valence bands (from −9.5 eV to the Fermi level) is mainly contributed by the Bp state, while that of the conduction bands come from both the Bp and Bep states. The Bes state also contributes to the DOS of the conduction band (above 4 eV), while making a very slight contribution to that of the valence band. The Bs state contributes to the lower part of the valence band (less than −7.5 eV) and to the upper part of the conduction band, especially in the 4 eV to 8 eV region of the total DOS. As discussed above, there is significant hybridization of the s and p states from both Be and B in the region of 4 eV to 8 eV, implying the tendency to form covalent bonds between Be and B atoms.
Figure 8 plots the total DOS for all stable phases at ambient pressure, corresponding to the Cmcm, , P63/mmc, Pmma and Pbam phases, from left to right. The dashed lines represent the position of the Fermi level. The first panel is the newly uncovered Cmcm phase, and the others are other known dynamically stable phases. Filling electrons at the Fermi level (approximately 1.18 states/eV/el.) shows that the new phase has an obvious metallic character, while the cubic phase with a band gap of 0.95 eV indicates its semiconductor property at low and intermediate pressures^{2}. Except for the phase, all other known phases are metallic, as shown in the last three panels of Figure 8.
Figure 9 shows electron density difference maps for the Cmcm phase on the selected slice (100) plane. It can be seen that electrons are gathered at the positions of the B atoms and especially between BoronBoron bonds, as indicated by the region in red in the top left panel and its enlarged bottom left panel. After removing the atoms, it is clearly seen that electrons are transferred from the Be atoms to the B atoms, as shown in the right two panels. From the electron gathering region between BoronBoron, one can speculate that there is a strong covalent interaction.
In order to give some insight into these bonding characters, an atomic and bond Mulliken population analysis, which can provide a good way to quantitatively evaluate the charge transfer chemical bond strength of the studied system, was performed and analyzed by the CASTEP code, with the results listed in Tables 7 and 8. From Table 7, it can be clearly seen that electrons transfer from the Be atoms to the B atoms in the Cmcm phase, as the charges for Be and B are 0.69 and −0.34, respectively.
Now let us turn to the bond Mulliken population analysis results. A high nonzero value of overlap population indicates that there is a strong covalent character of the bond, while a small value close to zero shows that there is weak or no interaction between two related atoms and a negative value indicates that the atoms cannot form a bond^{39}. From Table 8, it may be seen that the bond population ranges from 0.20 to 1.63 for the Cmcm phase. The maximum number, 1.63, exists between BoronBoron bonds, indicating their strong covalent character. However, the BeB bond has very weak covalence, as its Mulliken population is only 0.20. The population of BeBe is −0.24, suggesting that there are no bonds forming. All of these Mulliken population results are consistent with the conclusions drawn from the electron density difference maps. As discussed in the mechanical properties section of this work, the hardness of the Cmcm phase may be a result of the high population value of the BoronBoron bonds.
Some techniques such as the crystal orbital overlap population (COOP)^{40,41} and its analogous crystal orbital Hamilton population (COHP)^{42,43} can provide a straightforward view of orbitalpair interactions; based on these techniques, it is possible to analyze and interpret the bonding situation in solidstate materials. To elucidate the bonding situations in this new BeB_{2} phase, we performed crystal orbital Hamilton population (COHP) analysis, which partitions the band structure energy (in term of the orbital pair contributions) into bonding, nonbonding and antibonding energy regions within a specified energy range. Figure 10 shows the resulting –pCOHP as a function of energy for the new phase. Positive values of –pCOHP describe bonding energy regions, whereas negative values describe antibonding energy regions. As seen in the COHP diagrams in Figure 10, there appear to be obvious BeB bonding states at the Fermi level, while that is not the case for the BB combination, indicating that the interactions between BeB bonds in the unit cell are stronger than those of BB bonds, despite the fact that a single BeB bond is weaker than a single BB bond, as shown by the Mulliken population. Above or below the Fermi level (in the range of −6 to 6 eV), the COHP plots of the BeB and BB combinations are clearly dominated by bonding states, which shows that the new phase has a favorable stability performance.
Superconductivity Properties
Encouraged by the relatively simple binary MgB_{2} having a superconductivity transition temperature of 39 K^{44} and the controversy regarding the reported superconductivity properties of BeB_{2} and BeB_{2.75}^{19,21}, we also calculated the superconductivity properties of the Cmcm phase of BeB_{2}. The T_{c} can be estimated from the AllenDynes modified McMillan equation^{45}, which has been found to be highly accurate for materials with an EPC constant λ<1.5^{46}, where ω_{log} is the logarithmic average of the phonon frequency and μ* is the effective Coulomb repulsion and was assumed to be constant at 0.1. The calculated spectral function α^{2}F(ω) and integrated λ(ω) of the Cmcm phase are plotted in Figure 11. Our results reveal that the Cmcm phase exhibits fairly low superconductivity properties, with a T_{c} of only 0.1 K. These results shed light on the controversy regarding the reported superconductivity properties of BeB_{2} or BeB_{2.75}. The synthesized sample may contain both BeB_{2} and BeB_{2.75} phases. When the BeB_{2} phase dominates, an absence of superconductivity would be observed, as shown in Ref. [21], while when the BeB_{2.75} phase dominates, superconductivity appears.
Methods
Ab initio evolutionary simulations were run using the USPEX (Universal Structure Predictor: Evolutionary Xtallography) code^{47,48,49}.
The USPEX code depends on VASP (Vienna ab initio simulation package)^{50} to achieve global optimization to calculate the enthalpy of crystal structures and explore the lowest enthalpy phase of a given elemental composition. Here, we used the USPEX code to search for stable compounds and structures with a fixed chemical composition of Be_{n}B_{2n} (n = 1 to 5); the Cmcm phase comes from the 25th structure with the stoichiometry of Be_{2}B_{4}. During the structure search, USPEX selects a whole range of 50 generations to calculate, with each generation containing 50 individuals. The settings used for the variation operators are as follows: 60% of each generation was used to produce the next generation by heredity, 20% comes from soft mutations, 10% is produced randomly from space groups, and the rest is produced through lattice mutations. The minimum length of any lattice vector was defined as 2.0 Å. The cutoff for USPEX relaxation and the kpoints for resolution were 318 eV and 2π × 0.02 Å^{−1}, respectively.
Firstprinciples^{51} calculations were carried out using the density functional theory (DFT) approach by applying a generalized gradient approximation (GGA) for the exchange correlation functional^{52,53}. We applied the Ultrasoft pseudopotential introduced by Vanderbilt^{54}, and the kpoint samplings in the Brillouin zone were performed using the MonkhorstPack Scheme. The convergence tests used a kinetic energy cutoff of 600 eV and a kpoint of 13 × 7 × 8 for the predicted Cmcm phase in the geometry optimization calculations. The selfconsistent convergence of the total energy was 5 × 10^{−7} eV/atom, the maximum force on each atom was below 0.01 eV/Å and the maximum atomic displacement was below 5 × 10^{−4} Å. The phonon dispersion curves were plotted using the supercell calculation method^{55} applied in the Phonopy program^{56}. The calculation of the elastic constant and Mulliken overlap populations was carried out using the CASTEP code^{57}. From the calculated elastic constants C_{ij}, the polycrystalline corresponding bulk modulus B and shear modulus G were calculated using the VoigtReussHill approximation^{32,33}. In addition, Young's modulus E and Poisson's ratio σ were obtained by the equations E = (9G·B)/(3B + G), and σ = (3B−2G)/(6B + 2G), respectively.
In addition, we used three different methods to calculate hardness. These three methods were proposed by Xing Qiu Chen^{35}, Artem R. Oganov^{36} and Faming Gao et al.^{37,38}, respectively. The description of Chen's model can be found in the text. To use the formula of hardness given by Artem R. Oganov^{36}, we need to use the structure file POSCAR (which must contain an element symbol line) and set the parameters for goodBonds, valence and valence electrons. For main group elements, only the outermost electrons are considered as valence electrons under normal circumstances. Hence, the numbers of valence electrons for Be and B atoms are 2 and 3.
Details of Gao's model are described below. The Vickers hardness of complex crystals can be calculated by a geometric average of all bonds as follows, For the Cmcm phase, the total hardness is given by Because no dorbital valence electrons are involved in the chemical bonds, the hardness of each bond for Cmcm phase can be expressed by: where d^{u} is the length of the bond, is the valence electron density (which can be calculated by where Z_{Be} and Z_{B} are the valence electron numbers of the Be and B atoms constructing BeB or BB bonds, N_{Be} and N_{B} are the nearest coordination numbers of the Be and B atoms, N_{j} is the number of j bond in the unit cell, and V is the volume of the unit cell) and is the Phillips ionicity of the bond. According to the generalized ionicity scale, the Phillips ionicity can be obtained from the following formula, where f_{h} is the population ionicity scale of the chemical bond, p is the overlap population of the bonds, and p_{c} is the overlap population of the bonds in a specified pure covalent crystal (here 0.57 is adopted).
For the complex crystal compounds, we considered three effects on hardness: the covalent component, the ionic component and the small metallic component. First, we defined a factor of metallicity f_{m} as n_{m}/n_{e} for a simplestructured compound, where n_{m} and n_{e} are the numbers of electrons that can be excited at the ambient temperature and the total number of valence electrons in the unit cell, respectively. According to the electronic Fermi liquid theory, the thermally excited electron number n_{m} can be described by the product of D_{F} and the energy width kT, where k is the Boltzmann constant and T is the temperature. At the ambient temperature, kT is equal to 0.026 eV. Therefore, f_{m} can be written as: When the chemical bonds of a crystal are greater than or equal to two, we refer to it as a complex crystal. For the metallicity of complex crystals, the f_{m} can be calculated by where (or ) is the thermally excited electron number of Be or B atoms in the utype bond, N_{MA} (or N_{MB}) is the number of chemical bonds with a metallic component around Be or B atoms, and is the number of valence electrons per utype bond.
To elucidate the bonding information in this new phase, we adopted a variant of the familiar COHP approach that stems from a PW calculation and was dubbed “projected COHP” (pCOHP)^{58,59}. In this approach, all of the projection and analytic methods are implemented in a standalone computer program that processes PAW parameters and selfconsistent results from VASP.
The calculation of the electronphonon coupling (EPC) parameter λ was performed using the pseudopotential planewave method within the density functional perturbation theory (DFPT)^{60} as implemented in the Quantum Espresso package^{61} by using Von BarthCar type normconserving pseudopotential with cutoff energies of 80 and 320 Ry for the wave functions and the charge density, respectively. A 7 × 4 × 4 qpoint mesh in the first Brillouin zone was used in the EPC calculation.
Conclusions
In summary, a new stable phase of BeB_{2} with the space group of Cmcm was discovered by using ab initio evolutionary simulations. The Cmcm phase has a lower enthalpy than any previously proposed phase. The new structure is mechanically and dynamically stable, as determined by checking the calculated elastic constants and phonon dispersions, while several previously proposed phases (cubic: ; hexagonal: P6/mmm; orthorhombic: Imma) were found to be dynamically unstable. The Cmcm phase may transform to the cubic phase when the pressure exceeds 13 GPa. The calculated electronic band structure and density of state suggest that the uncovered new phase is metallic. Scattered hardness values calculated from three models suggest the complex electronic and bonding features of the Cmcm phase. The charge density difference maps and the Mulliken population analysis reveal that there are strong covalent interactions between the B atoms. The COHP diagrams show that the total interaction of BeB bonds is stronger than that of BB bonds. The Cmcm phase exhibits fairly low superconductivity properties, with a calculated T_{c} of approximately 0.1 K. The current theoretical predictions will most likely promote further experimental and theoretical investigation on the BeB system.
Change history
27 February 2015
A correction has been published and is appended to both the HTML and PDF versions of this paper. The error has been fixed in the paper.
References
 1.
Luo, F. et al. Ab initio calculation of lattice dynamics and thermodynamic properties of beryllium. J. Appl. Phys. 111, 053503 (2012).
 2.
Hermann, A., Ashcroft, N. W. & Hoffmann, R. Binary Compounds of Boron and Beryllium A Rich Structural Arena with Space for Predictions. Chem. Eur. J. 19, 4184–4197 (2013).
 3.
Kádas, K., Vitos, L., Johansson, B. & Kollár, J. Structural stability of βberyllium. Phys. Rev. B. 75, 035132 (2007).
 4.
Kádas, K. et al. Temperaturedependent elastic properties of αberyllium from first principles. Phys. Rev. B. 76, 235109 (2007).
 5.
Robert, G., Legrand, P. & Bernard, S. Multiphase equation of state and elastic moduli of solid beryllium from first principles. Phys. Rev. B. 82, 104118 (2010).
 6.
Oberkofler, M., Reinelt, M. & Linsmeier, C. Quantum Modeling of Hydrogen Retention in Beryllium Bulk and Vacancies. J. Phys. Chem. C. 114, 3588–3598 (2010).
 7.
Xia, Y., Li, Q. & Ma, Y. M. Novel superhard polymorphs of Be_{3}N_{2} predicted by firstprinciples. Comput. Mat. Sci. 49, S76–S79 (2010).
 8.
Federici, G. et al. Plasmamaterial interactions in current tokamaks and their implications for the next step fusion reactors. Nucl. Fusion. 41, 1967–2137 (2001).
 9.
Eremets, M. I., Struzhkin, V. V., Mao, H. K. & Hemley, R. J. Superconductivity in Boron. Science. 293, 272–274 (2001).
 10.
Will, G. & Kiefer, B. Electron deformation density in rhombohedral αBoron. Anorg. Allg. Chem. 627, 2100–2104 (2001).
 11.
Cumberland, R. W. et al. Osmium Diboride, An UltraIncompressible, Hard Material. J. Am. Chem. Soc. 127, 7264–7265 (2005).
 12.
Wang, D. Y., Wang, B. & Wang, Y. X. New crystal structure of IrB and IrB_{2}: Firstprinciples calculations. J. Phys. Chem. C. 116, 21961–21966 (2012).
 13.
Wang, Y. X. Elastic and electronic properties of TcB_{2} and superhard ReB_{2}: Firstprinciples calculation. Appl. Phys. Lett. 91, 101904 (2007).
 14.
Guo, X. J. et al. Bond ionicities and hardness of B_{13}C_{2}like structured B_{y}X crystals (X = C, N, O, P, As). Phys. Rev. B. 73, 104115 (2006).
 15.
Liu, Z. Y. et al. Prediction of a sandwichlike conducting superhard boron carbide: Firstprinciples calculations. Phys. Rev. B. 73, 172101 (2006).
 16.
Hu, Q. K. et al. Firstprinciples studies of structural and electronic properties of hexagonal BC_{5}. Phys. Rev. B. 73, 214116 (2006).
 17.
Shein, I. R. & Ivanovskii, A. L. Superconductivity in Be_{2}B? Comparative analysis of the band structure of MgB_{2}, BeB_{2} and Be_{2}B. Phys. Stat. Sol. B. 227, R1–R3 (2001).
 18.
Sands, D. E., Cline, C. F., Zalkin, A. & Hoenig, C. L. The berylliumboron system. Acta Crystallogr. 14, 309–310 (1961).
 19.
Young, D. P. et al. Superconducting properties of BeB_{2.75}. Phys. Rev. B. 65, 180518 (2002).
 20.
Hermann, A., Ashcroft, N. W. & Hoffmann, R. Making Sense of BoronRich Binary Be–B Phases. Inorg. Chem. 51, 9066–9075 (2012).
 21.
Felner, I. Absence of superconductivity in BeB_{2}. Physica C. 353, 11–13 (2001).
 22.
Profeta, G., Continenza, A., Bernardini, F. & Massidda, S. MgB_{2} and BeB_{2}: A comparative study of their electronic and superconducting properties. Phys. Rev. B. 65, 054502 (2001).
 23.
Islam, A. K. M. A. et al. Elastic and electronic properties of BeB_{2} in comparison to superconducting MgB_{2} and NbB_{2}. Solid State Commu. 139, 315–320 (2006).
 24.
Rivillo, T. & Wallace, W. E. Magnetism and Phase Relations of the PrAl_{2}CaAl_{2} and GdAl_{2}CaAl_{2} Systems. J. Solid State Chem. 33, 309–315 (1980).
 25.
Iandelli, A. MX_{2}Verbindungen der Erdalkali und Seltenen Erdmetalle mit Gallium, Indium und Thallium. Z. Anorg. Allg. Chem. 330, 221–232 (1964).
 26.
Nuspl, G., Polborn, K., Evers, J., Landrum, G. A. & Hoffmann, R. The FourConnected Net in the CeCu_{2} Structure and Its Ternary Derivatives. Its Electronic and Structural Properties. Inorg. Chem. 35, 6922–6932 (1996).
 27.
Cordier, G., Czech, E. & Schafer, H. Z. On SrAl_{2}, a high pressure phase. Naturforsch. B. 37, 1442–1445 (1982).
 28.
Smith, G. S., Mucker, K. F., Johnson, Q. & Wood, D. H. The crystal structure of Ga_{2}Mg. Acta Crystallogr. B. 25, 549–553 (1969).
 29.
Qian, G. R. et al. Variable cell nudged elastic band method for studying solidsolid structural phase transitions. Comput. Phys. Commun. 184, 2111–2118 (2013).
 30.
Fan, C. Z. et al. Potential superhard osmium dinitride with fluorite and pyrite structure: Firstprinciples calculations. Phys. Rev. B. 74, 125118 (2006).
 31.
Born, M. On the stability of crystal lattices. I. Proc. Cambridge Philos. Soc. 36, 160–172 (1940).
 32.
Hill, R. The Elastic Behaviour of a Crystalline Aggregate. Proc. Phys. Soc. A 65, 349–354 (1951).
 33.
Reuss, A. Berechnung der Fliessgrenze von Mischkristallen auf Grund der Plastizitatsbedingung fur Einkristalle. Z. Angew. Math. Mech. 9, 49–58 (1929).
 34.
Pugh, S. F. Relations between the elastic moduli and the plastic properties of polycrystalline pure metals. Philos. Mag. 45, 823–843 (1954).
 35.
Chen, X. Q. et al. Hardness of T carbon : Density functional theory calculations. Phys. Rev. B. 84, 121405 (2011).
 36.
Lyakhov, A. O. & Oganov, A. R. Evolutionary search for superhard materials: Methodology and applications to forms of carbon and TiO_{2}. Phys. Rev. B. 84, 092103 (2011).
 37.
Gao, F. M. et al. Hardness of Covalent Crystals. Phys. Rev. Lett. 91, 015502 (2003).
 38.
Guo, X. J., Li, L. & L, Z. Y. Hardness of covalent compounds: Roles of metallic component and d valence electrons. J. Appl. Phys. 104, 023503 (2008).
 39.
Segall, M. D., Shah, R., Pichard, C. J. & Payne, M. C. Population analysis of planewave electronic structure calculations of bulk materials. Phys. Rev. B. 54, 16317–16320 (1996).
 40.
Hughbanks, T. & Hoffmann, R. Chains of TransEdgeSharing Molybdenum Octahedra: MetalMetal Bonding in Extended Systems. J. Am. Chem. Soc. 105, 3528 (1983).
 41.
Hoffmann, R. Solids and Surfaces: A Chemist′s View of Bonding in Extended Structures (VCH publishers Inc., New York, 1988).
 42.
Dronskowski, R. Computational chemistry of Solid State Material (WileyVCH: Weinheim, New York, 2005).
 43.
Dronskowski, R. & Blöchl, P. E. Crystal Orbital Hamilton Populations (COHP). EnergyResolved Visualization of Chemical Bonding in Solids Based on DensityFunctional Calculations. J. Phys. Chem. 97, 8617–8624 (1993).
 44.
Nagamatsu, J. et al. Superconductivity at 39 K in magnesium diboride. Nature. 410, 63–64 (2001).
 45.
Allen, P. B. & Dynes, R. C. Transition temperature of strongcoupled superconductors reanalyzed. Phys. Rev. B. 12, 9051975 (1975).
 46.
Jin, X. et al. Superconducting highpressure phases of disilane. Proc. Natl. Acad. Sci. USA. 107, 9969–9973 (2010).
 47.
Oganov, A. R. & Glass, C. W. Evolutionary crystal structure prediction as a tool in materials design. J. Phys.:Condens. Matter. 20, 064210 (2008).
 48.
Glass, C. W., Oganov, A. R. & Hansen, N. USPEX—Evolutionary crystal structure prediction. Comput. Phys. Commun. 175, 713–720 (2006).
 49.
Lyakhov, A. O., Oganov, A. R., Stokes, H. T. & Zhu, Q. New developments in evolutionary structure prediction algorithm USPEX. Comput. Phys. Commun. 184, 1172–1182 (2013).
 50.
Kresse, G. & Furthmüller, J. Efficient iterative schemes for ab initio totalenergy calculations using a planewave basis set. Phys. Rev. B. 54, 11169–11186 (1996).
 51.
Gillan, M. J. et al. Firstprinciples modelling of Earth and planetary materials at high pressures and temperatures. Rep. Prog. Phys. 69, 2365–2441 (2006).
 52.
Perdew, J. P. et al. Atoms, molecules, solids, and surfaces: Applications of the generalized gradient approximation for exchange and correlation. Phys. Rev. B. 46, 6671–6687 (1992).
 53.
Perdew, J. P., Burke, K. & Ernzerhof, M. Generalized Gradient Approximation Made Simple. Phys. Rev. Lett. 77, 3865–3868 (1996).
 54.
Vanderbilt, D. Soft selfconsistent pseudopotentials in a generalized eigenvalue formalism. Phys. Rev. B. 41, 7892–7895 (1990).
 55.
Frank, W., Elsässer, C. & Fähnle, M. Ab initio ForceConstant Method for Phonon Dispersions in Alkali Metals. Phys. Rev. Lett. 74, 1791–1794 (1995).
 56.
Parlinski, K., Li, Z. Q. & Kawazoe, Y. FirstPrinciples Determination of the Soft Mode in Cubic ZrO_{2}. Phys. Rev. Lett. 78, 4063–4066 (1997).
 57.
Segall, M. D. et al. Firstprinciples simulation ideas, illustrations and the CASTEP code. J. Phys.: Condens. Matter. 14, 2717–2744 (2002).
 58.
Deringer, V. L., Tchougréeff, A. L. & Dronskowski, R. Crystal Orbital Hamilton Population (COHP) Analysis As Projected from PlaneWave Basis Sets. J. Phys. Chem. A 115, 5461–5466 (2011).
 59.
Maintz, S., Deringer, V. L., Tchougréeff, A. L. & Dronskowski, R. Analytic Projection From PlaneWave and PAW Wavefunctions and Application to ChemicalBonding Analysis in Solids. J. Comput. Chem. 34, 2557–2567 (2013).
 60.
Gonze, X. & Lee, C. Dynamical matrices, born effective charges, dielectric permittivity tensors, and interatomic force constants from densityfunctional perturbation theory. Phys. Rev. B. 55, 10355 (1997).
 61.
Giannozzi, P. et al. QUANTUM ESPRESSO: a modular and opensource software project for quantum simulations of materials. J. Phys.: Condens. Matter. 21, 395502 (2009).
Acknowledgements
This work was supported by the Research Foundation of Education Bureau of Hebei Province (ZD20131039), the Natural Science Foundation of Hebei Province (E2014203243) and the NSFC (Grant No. 51121061), which is gratefully acknowledged.
Author information
Affiliations
State Key Laboratory of Metastable Materials Science and Technology, Yanshan University, Qinhuangdao 066004, China
 Changzeng Fan
 , Ye Jin
 , Jian Li
 & Xu Dong
Authors
Search for Changzeng Fan in:
Search for Ye Jin in:
Search for Jian Li in:
Search for Xu Dong in:
Contributions
C.Z.F. conceived the idea. Y.J. performed the ab initio evolutionary simulations and DFT calculations. Y.J. and J.L. carried out the hardness predictions. J.L. did the COHP analysis. X.D. performed the superconductivity properties calculations. C.Z.F.and Y.J. wrote the manuscript with contributions from all.
Competing interests
The authors declare no competing financial interests.
Corresponding author
Correspondence to Changzeng Fan.
Rights and permissions
This work is licensed under a Creative Commons Attribution 4.0 International License. The images or other third party material in this article are included in the article's Creative Commons license, unless indicated otherwise in the credit line; if the material is not included under the Creative Commons license, users will need to obtain permission from the license holder in order to reproduce the material. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/
About this article
Further reading

Prediction of the fundamental properties of novel BeBTabased ternary compounds from firstprinciples calculations
Physical Review Materials (2019)

Density functional theory study on structure and stability of BeBn + clusters
Rapid Communications in Mass Spectrometry (2017)

PressureInduced Stable Beryllium Peroxide
Inorganic Chemistry (2017)

Coexistence of Superconductivity and Superhardness in Beryllium Hexaboride Driven by Inherent Multicenter Bonding
The Journal of Physical Chemistry Letters (2016)

Exploration of stable stoichiometries, physical properties and hardness in the Rh–Si system: a firstprinciples study
RSC Advances (2015)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.